DETERMINATION OF THE LONG-TERM PROPERTIES FOR MIRAGRID
Prepared by: TenCate Geosynthetics Americas 365 South Holland Drive Pendergrass, GA 30567 Tel 706 693 2226 Fax 706 693 4400 www.tencate.com August 12, 2014
Miragrid 5XT in SRW
Miragrid geogrids are the leading polyester geogrids used for soil reinforcement applications. Starting in the late 1980s, extensive research and testing have been performed on Miragrid
geogrids to determine the long term, in-situ properties.
This technical note describes each of the relevant properties in detail and the appropriate testing conducted on Miragrid geogrids.
Miragrid geogrids are high strength, high tenacity polyester geogrids in a full range of tensile strengths. Miragrid geogrids are woven and then coated with a PVC coating to provide dimensional stability. Miragrid geogrids are used in a wide variety of soil reinforcement applications including internally reinforced soil walls, segmental retaining wall reinforcement, steep reinforced slopes, and reinforcement in a variety of landfill applications including potential voids bridging and veneer stability. Applications where long term design strength is necessary for the stability of the structure are ideal applications where Miragrid geogrids can be used.
Standard roll dimensions for
Miragrid geogrids are
Standard Roll Dimensions
Width x Length m (ft)
Roll Area m2 (yd2)
2XT 1.8 (6.0) x 45.7 (150) 82.3 (100)
3XT 1.8 (6.0) x 45.7 (150) 3.6 (12) x 45.7 (150)
82.3 (100) 164.5 (200)
5XT 1.8 (6.0) x 45.7 (150) 3.6 (12) x 45.7 (150)
82.3 (100) 164.5 (200)
7XT 1.8 (6.0) x 45.7 (150) 3.6 (12) x 61 (200)
82.3 (100) 220 (267)
8XT 1.8 (6.0) x 45.7 (150) 3.6 (12) x 61 (200)
82.3 (100) 220 (267)
10XT 3.6 (12) x 61 (200) 220 (267)
20XT 3.6 (12) x 61 (200) 220 (267)
22XT 3.6 (12) x 61 (200) 220 (267)
24XT 3.6 (12) x 61 (200) 220 (267)
Polymer type and grade
Miragrid geogrids are produced from high molecular weight, low CEG, high tenacity polyester (PET) yarns with the following physical properties:
Minimum Average Molecular Weight 25,000
Carboxyl End Groups
Conventional Creep Testing of Miragrid Geogrids
Figure 2: Wide Width Tensile Test of Miragrid
The testing of Miragrid geogrids is carried out under controlled conditions including the following:
Overall management of process control is governed by documented procedures.
Documented test methods and work instructions govern the comprehensive inspection and testing of each lot.
Testing equipment is selected based upon needs and the ability to satisfy specified requirements with the equipment being suitably maintained.
Training of personnel is adequate and documented.
Appropriate Quality Records are maintained.
Each sample to be tested is accompanied with a label for the particular manufacturing roll number. Test results are recorded on Quality Control Test Reports by number and then entered into a computer database by roll number.
Once the sample has been delivered to the Quality Control lab, the sample is tested. The standard operating procedure for each test is documented with copies of the appropriate test procedure on file in the Quality Control laboratory. The preparation for each sample is conducted in accordance with Standard Operating Procedures and ASTM requirements. Creep Reduction Factor, RFCR All polymers used in the manufacture of geosynthetics are subject to sustained load deformation or creep . Creep behavior is a function of stress level, time, temperature (environment), and molecular structure . The reduction factor for creep, RFCR, is used to limit the magnitude of creep at specified strain levels over a specific time period.
There are three methods for measuring
geosynthetic creep: Conventional Creep Testing, Time-temperature Superposition (TTS), and Stepped Isothermal Method (SIM) . The validation of the creep factors currently used for Miragrid geogrids is based on conventional and Stepped Isothermal creep rupture data generated in compliance with Washington DOT T925 test procedure and NHI (National Highway Institute) guidelines. This test data demonstrate that loads of at least 63.17% (RFCR = 1.58) of the ultimate tensile strength (per ASTM D 6637) is reasonable for use with Miragrid geogrids .
Durability Reduction Factor, RFD
Geosynthetics, like all other construction materials, slowly degrade over time. The rate of degradation depends on the molecular make-up of the geosynthetic polymer and the nature of the environment to which the geosynthetic is exposed. Since most geosynthetics are buried in non-aggressive soil environments, geosynthetic degradation normally occurs at a very slow, almost unmeasureable, rate. Still, it is possible for significant rates of degradation to take place if unstable polymers are used or extreme conditions are encountered as described in subsequent sections.
The partial reduction factor for durability, RFD, is derived from testing. Figure 4 compiles the reduction factors associated with durability testing reported . These reduction factors are compared with the more conservative FHWA/Industry guidelines . TenCate geosynthetics were included in several of the referenced tests. Figure 4. Durability Reduction Factors, RFD, for High Strength Geosynthetics @ 75 Years
1 1.1 1.2 1.3 1.4 1.5
Durability Reduction Factor, RFD
Average Reduction Factors, RFD, from Testing High-Strength PET
FHWA/Industry Guidelines for PET in the Absence of Product-Specific Testing
Max. Reduction Factors, RFD, from Testing PP & PE and FHWA/Industry Guidelines for PP & PP
Typical Range of Soil pH
Default partial reduction factors for durability, RFD , are recommended where polymer stability can be demonstrated and where the anticipated soil environment is non-aggressive. FHWA has given some conservative guidance on the selection of the RFD in the absence of product-specific testing . Yet, specific product testing and field experience has demonstrated that the RFD value shown in the table below are commonly applicable to polyester geotextiles and coated geogrids as long as minimum molecular weight and maximum number Carboxyl End Groups are maintained. Recommended RFD for Miragrid Geogrids in Typical Soils
Geosynthetic Type Minimum PET Yarn Criteria RFD
Woven Polyester (PET) Geotextiles
Woven/Coated Polyester (PET) Geogrids
Each report contains summary tables that list the retained product strength and the calculated reduction factor per soil type . The testing program was as follows:
A lightweight geogrid (Miragrid 3XT) was tested in three soil types with d50 values of 0.3mm, 4.5 mm, and to 22mm.
The heaviest geogrid (Miragrid 24XT) was tested in two soil types with a d50 of 4.5mm and 42 mm.
Medium weight geogrids (Miragrid 5XT, Miragrid 8XT, and Miragrid 10XT) were tested in tested in three soil types with d50 values of 0.3mm, 4.5 mm, and to 22mm.
An additional medium weight geogrid (Miragrid 7XT) was tested in two soil types with d50 values of 0.3mm and 4.5 mm.
The strength reduction factors to account for installation damage to the reinforcement, RFID, for the Miragrid geogrids are shown below.
Soil Type 2XT 3XT 5XT 7XT 8XT
Type 3 (Sand, Silt, Clay) 1.05 1.05 1.05 1.05 1.05
Type 2 (Sandy Gravel) 1.10 1.10 1.10 1.10 1.10
Type 1 (Gravel) 1.25 1.25 1.25 1.25 1.25
Soil Type 10XT 20XT 22XT 24XT
Type 3 (Sand, Silt, Clay) 1.05 1.05 1.05 1.05
Type 2 (Sandy Gravel) 1.10 1.10 1.10 1.10
Type 1 (Gravel) 1.25 1.25 1.25 1.25
Interaction Coefficients for Pullout and Sliding
Reinforcement applications using geosynthetics require an estimate of two interaction coefficients . The Coefficient of Shear Stress Interaction (Ci) is required to calculate the reinforcement pullout capacity of the geosynthetic . The Coefficient of Direct Sliding (Cds) is required to calculate the resistance to internal sliding generated along the surface of the geosynthetic .
The Coefficient of Shear Stress Interaction, Ci, and Coefficient of Direct Sliding, Cds, for Miragrid geogrids were determined from independent testing   and are as follows:
Soil Type U.S.C.S. Ci Cds
Silty clay, sandy clay, clayey silt (ML, CL) 0.7 0.8 0.7
Silty sands, fine to medium sands (SM, SP, SW) 0.8 0.9 0.8
Dense well-graded sand, sand and gravel
(SW, GP, GW) 0.9 1.0 0.9
Extensive research has been conducted on the interaction properties of Miragrid geogrids. A research paper entitled Soil Interaction Characteristics of Geotextiles and Geogrids by Koutsourais, Sandri, and Swan  and actual testing by Geosynthec Consultants  on Miragrid geogrids in a concrete sand provide detailed evidence verifying the values listed above. UV Resistance Sunlight is an important cause of degradation to all organic materials, including polymers from which geosynthetics are produced . Of the three types of energy produced from the sun, ultraviolet (UV) is the most